R. O. Ajemba and O. D. Onukwuli / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 5, September- October 2012, pp.732-742

Determination Of The Optimum Dissolution Conditions Of Ukpor Clay In Hydrochloric Acid Using Response Surface Methodology R. O. Ajemba and O. D. Onukwuli Department of Chemical Engineering, Nnamdi Azikiwe University, P. M. B. 5025, Awka, Anambra State, Nigeria

ABSTRACT Ukpor clay was dissolved in solutions of hydrochloric acid to investigate its dissolution rate. Response surface methodology was employed to determine the optimum conditions for the dissolution. The experiments were performed within the ranges of the process variables as mentioned herein: 400 – 8000C for calcination temperature; 0.5 – 4 mol/L for acid concentration; 0.02 – 0.10 g/ml for clay to acid ratio; 60 – 1200C for reaction temperature; and 90 to 720 rpm for stirring speed. The analysis of variance indicated that a second order polynomial regression equation was appropriate for fitting the experimental data. The experimental confirmation tests showed a correlation between the predicted and experimental response values (R2 = 0.9400). The optimum conditions for the process variables were obtained as: 6680C for calcination temperature; 2.93mol/l for acid concentration; 0.027g/ml for clay to acid ratio; 107 0C for reaction temperature; and 368rpm for stirring speed. Under these conditions the dissolution rate was 97.85%.

Keywords: Optimization; calcination; dissolution; hydrochloric acid; ANOVA; clay

1. INTRODUCTION Clay dissolution in acid medium is gaining serious academic attention in the recent time. This is as a result of the need of a low cost source of metallic ores. Clay is a well known aluminous and siliceous material from which the metallic ions can be replaced by the hydrogen ions from inorganic acids. Metallic ions such as Al3+, Fe3+, Mg2+, and sometimes Mn2+ can be extracted from the clay mineral by dissolution in acid mediums. Dissolution of various metal ores in different acidic media has been investigated by a great number of authors [1 – 7]. Depending on the extent of acid dissolution, the resulting solid product contains unaltered layers and amorphous three-dimensional cross-linked silica, while the ambient acid solution contains ions according to the chemical composition of the clay and acid used. The extent of the dissolution reaction depends on both clay

mineral type and reaction conditions, such as the acid/clay ratio, acid concentration, time and temperature of the reaction [8 – 10]. Most of the reports in the literature on dissolution of ores in acidic media were conducted using the conventional method of investigation, by varying one factor whilst maintaining all other factors constant. This conventional method is cumbersome and time consuming and has low efficiency when it comes to optimizing the process [11, 12]. Process factors do interact with each other, but this interaction cannot be investigated using the conventional method. Response surface methodology (RSM) technique helps in overcoming the limitations of the conventional method of analysis. The main objective of RSM is to check the optimum operational conditions for a given system and determine a region that satisfies the operational specifications [13]. It helps in obtaining a second-order polynomial prediction equation or some other mathematical equations to describe the experimental data obtained at some particular combinations of the input variables. In this work, the determination of the optimum extraction of Al3+ ion which is one of the most important metal ores present in clay minerals and can be extracted by dissolution is the target. The clay mineral from Ukpor will be calcined before dissolution in hydrochloric acid and RSM will be used to optimize the dissolution parameters, thereby ensuring high dissolution efficiency and determining the interactive effects of the calcination temperature, reaction temperature, acid concentration, particle size, clay/acid ratio, and stirring speed on the dissolution process.

2. MATERIALS AND METHODS The clay samples from Ukpor was mined from the region and separated from dirt that contaminated them. The mined clay was wet and was sun-dried for three days after which the dried sample was grinded with mortar and sieved with 75µm sieve size. The sieved samples were then calcined in a furnace with a temperature range of 1000C to 12000C. The calcination temperature was chosen in the range of 5000C to 8000C for all the samples. The calcination time was also varied between 0.3 to 8 hours. The clay was characterized

732 | P a g e

R. O. Ajemba and O. D. Onukwuli / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 5, September- October 2012, pp.732-742 with X-ray fluorescence to ascertain the chemical composition. 2.1.

Dissolution experiment The calcined samples were then ground and sieved into various particle sizes and labeled accordingly. For each experiment, 10 g of the sized fractions was weighed out and reacted with already determined volume of the acids in a 250 ml bottomed flask. The flask and its contents were heated to a fixed temperature of 700C while on a magnetic stirring plate and stirring was continued throughout the reaction duration. Also the reactor was fitted with a condenser to prevent losses by evaporation. After the reaction time was completed, the suspension was immediately filtered to separate un-dissolved materials, washed three times with distilled water. The resulting solutions were diluted and analyzed for aluminum ion using MS Atomic Absorption Spectrophotometer. The residue was also collected, washed to neutrality with distilled water, air dried and oven dried at 600C and then reweighed. The difference in weight was noted for determining the fraction of the alumina ore that dissolved. 2.2. Design of Experiment The process variables affecting the dissolution of Ukpor clay in sulphuric acid were investigated using RSM combined with five-level, five-factor

fractional factorial design as established by Design Expert software (8.0.1 trial version). The process variables were calcination temperature of 500 – 8000C, reaction temperature of 60 – 1200C, acid concentration of 0.5 – 4mol/l, solid/liquid ratio of 0.02 – 0.10g/ml, and stirring speed of 90 – 720rpm. The response variable was chosen as % yield of alumina. The factor levels were coded as –α, - 1, 0, +1 and +α. The range and levels are shown in Table 1. A total of 31 runs were carried out to optimize the process variables and experiments were performed according to the actual experimental design matrix shown in Table 2. The experiments were performed randomly to avoid systemic error. The results were analyzed using the coefficient of determination, analysis of variance (ANOVA), and response plots. In RSM, the most widely used second-order polynomial equation developed to fit the experimental data and identify the relevant model terms may be written as: Y = β0 + ∑βi xi + ∑βii xii2 + ∑βij xi xj + ε (1) Where Y is the predicted response variable, in this study the % yield of alumina, β0 is the constant coefficient, βi is the ith linear coefficient of the input variable xi, βii is the ith quadratic coefficient of the input variable xi, βij is the different interaction coefficients between the input variables xi and xj, and ε is the error of the model.

Table 1: Experimental range of the independent variables, with different levels, to study alumina production during the dissolution of local clays in sulphuric, hydrochloric, and nitric acids Independent variable Symbol Range and levels -α -1 0 +1 +α Calcination temp (0C) X1 350 500 650 800 950 Leaching temp. (0C) X2 30 60 90 120 150 Acid Conc. (mol/l) X3 -1.25 0.5 2.25 4.0 5.75 S/L Ratio (g/l) X4 0.01 0.02 0.03 0.04 0.05 Stirring Rate (rpm) X5 -225 90 315 720 1035

Run order 1 2 3 4 5 6 7 8 9 10 11 12 13

Calcin (0C), X1 Coded -1 +1 -1 +1 -1 +1 -1 +1 -1 +1 -1 +1 -1

Table 2: Experimental design/plan for alumina leaching from local clays Temp Leach Temp Acid Conc. Solid/Liquid Stirring Speed (0C), X2 (mol/l), X3 Ratio (g/l), X4 (rpm), X5 Real Coded Real Coded Real Coded Real Coded Real 500 -1 60 -1 0.5 -1 0.02 +1 720 800 -1 60 -1 0.5 -1 0.02 -1 90 500 +1 120 -1 0.5 -1 0.02 -1 90 800 +1 120 -1 0.5 -1 0.02 +1 720 500 -1 60 +1 4.0 -1 0.02 -1 90 800 -1 60 +1 4.0 -1 0.02 +1 720 500 +1 120 +1 4.0 -1 0.02 +1 720 800 +1 120 +1 4.0 -1 0.02 -1 90 500 -1 60 -1 0.5 +1 0.04 -1 90 800 -1 60 -1 0.5 +1 0.04 +1 720 500 +1 120 -1 0.5 +1 0.04 +1 720 800 +1 120 -1 0.5 +1 0.04 -1 90 500 -1 60 +1 4.0 +1 0.04 +1 720

% Yield Exp. 34.8 57.8 42.6 65.0 39.6 55.4 50.7 67.0 33.7 37.5 40.2 59.0 44.9

Pred. 36.3 54.4 41.0 63.7 40.5 56.5 53.6 65.0 31.0 35.1 39.6 53.5 46.7

733 | P a g e

R. O. Ajemba and O. D. Onukwuli / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 5, September- October 2012, pp.732-742 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31

+1 -1 +1 -2 +2 0 0 0 0 0 0 0 0 0 0 0 0 0

800 500 800 350 950 650 650 650 650 650 650 650 650 650 650 650 650 650

-1 +1 +1 0 0 -2 +2 0 0 0 0 0 0 0 0 0 0 0

60 120 120 90 90 30 150 90 90 90 90 90 90 90 90 90 90 90

+1 +1 +1 0 0 0 0 -2 +2 0 0 0 0 0 0 0 0 0

3. RESULTS AND DISCUSSIONS 3.1.

Characterization The results of the X-ray fluorescence analysis are shown in Table 3. The results show that Ukpor clay is composed of mainly silica, alumina and iron oxides, and other trace oxides like calcium oxide, magnesium oxide, titanium oxide, potassium oxide and others. Table 3: Chemical composition of Ukpor clay determined by XRF Chemical constituent Composition (%) Al2O3 26.9 SiO2 48.6 Fe2O3 17.13 CaO 0.08 MnO 0.003 MgO 0.329 P2O5 0.2 TiO2 2.06 V2O5 0.14 CuO 0.064 ZnO 0.008 Rb2O 1.15 Loss on ignition (LOI) 3.05 3.2.

Statistical Analysis The second-order model tested at the 95% confidence level obtained for extraction of Al 2O3 from Ukpor clay is as follows: YAl2O3 = 69.37 + 6.56X1 + 5.02X2 + 3.83X3 – 3.23X4 + 1.41X5 + 2.06X1X2 – 0.78X1X3 – 1.97X1X4 – 1.05X1X5 – 0.09X2X3 + 0.57X2X4 + 0.88X2X5 + 1.31X3X4 + 2.07X3X5 + 0.26X4X5 – 3.95X12 – 3.08X22 – 2.95X32 – 4.90X42 – 6.33X52 (3) The results were analyzed by using ANOVA i.e. analysis of variance suitable for experimental

4.0 4.0 4.0 2.25 2.25 2.25 2.25 -1.25 5.75 2.25 2.25 2.25 2.25 2.25 2.25 2.25 2.25 2.25

+1 +1 +1 0 0 0 0 0 0 -2 +2 0 0 0 0 0 0 0

0.04 0.04 0.04 0.03 0.03 0.03 0.03 0.03 0.03 0.01 0.05 0.03 0.03 0.03 0.03 0.03 0.03 0.03

-1 -1 +1 0 0 0 0 0 0 0 0 -2 +2 0 0 0 0 0

90 90 720 405 405 405 405 405 405 405 405 -225 1035 405 405 405 405 405

47.6 45.3 66.0 43.0 60.0 46.0 64.0 44.0 67.0 57.4 38.0 34.0 50.0 71.0 69.0 70.0 70.0 71.0

44.5 44.0 65.0 40.4 66.7 47.0 67.1 49.9 65.2 56.2 43.3 41.2 46.9 69.4 69.4 69.4 69.4 69.4

design used and shown in Table 4. The ANOVA of the quadratic regression model indicates that the model is significant. The model F-value of 7.83 implied the model to be significant. Model F-value was calculated as ratio of Adj. mean square of the regression and Adj. mean square of the residual. The model P-value (Prob. > F) is very low which reiterates the model significant. The P-values were used as a tool to check the significance of each of the model coefficients. These values are all given in Table 3. The smaller the P-value the more significant is the corresponding coefficient. Values of P < 0.05 indicate the model terms to be significant. In Table 3, the values of P for the coefficients estimated indicate that among the tested variables used in the design, X1, X2, X3, X4, X12, X22, X32, X42 and X52 (where X1 = Calcination temperature, X2 = leaching temperature, X3 = acid concentration, X4 = stirring rate, and X5 = liquid/solid ratio,) are significant model terms. The model equation with the significant coefficients is shown in Equation (4). Y = 69.37 + 6.56X1 + 5.02X2 + 3.83X3 – 3.23X4 – 3.95X12 – 3.08X22 – 2.95X32 – 4.90X42 – 6.33X52 (4) In terms of the actual factors the model equation is as follows: % YieldAl2O3 = - 30.96 + 0.09 * Calcination temperature + 0.60 * leaching temperature + 6.53 * acid concentration + 0.05 * Stirring rate – 5.08 * Calcination temperature2 – 3.07 * Leaching Temperature2 – 1.16 * Acid Concentration2 – 4.04 * stirring rate2 – 35355.45 * Solid/Liquid ratio2 (5) The coefficient of regression (R2), calculated as the ratio of the regression sum of squares to the total sum of squares, was found to be 0.9400, this indicates that 94.00% of the variability in the yield data is explained by the regression model, showing a very good fit of the model. The S-value of 0.2471 and R-Sq (adj.) value of 0.8200 indicates a better fitting model. S is the square root of the error mean

734 | P a g e

R. O. Ajemba and O. D. Onukwuli / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 5, September- October 2012, pp.732-742 square, MSE, and represents the “standard error of the model” and a lower value of S indicates a

Source Model X1 X2 X3 X4 X5 X 1X 2 X 1X 3 X 1X 4 X 1X 5 X 2X 3 X 2X 4 X 2X 5 X 3X 4 X 3X 5 X 4X 5 X 12 X 22 X 32 X 42 X 52 Residual Lack of fit Pure Error Cor. Total

fitting model. R-Sq (adj.) indicates how well the model fits the observed data.

Table 4: ANOVA for response surface quadratic model Coefficient Sum of Degree of F-value Estimate Squares Freedom 69.37 4531.55 20 7.83 6.56 326.30 1 59.19 5.02 225.38 1 40.89 3.83 308.92 1 56.04 -3.23 46.42 1 8.42 1.41 118.71 1 21.53 2.06 0.48 1 0.086 -0.78 4.58 1 0.83 -1.97 12.63 1 2.29 -1.06 8.72 1 1.58 -0.09 13.13 1 2.38 0.57 0.26 1 0.048 0.88 0.11 1 0.020 1.31 0.0028 1 0.0005 2.07 0.69 1 0.13 0.26 6.39 1 1.16 -3.95 211.95 1 38.45 -3.08 392.53 1 71.21 -2.95 644.27 1 116.88 -4.90 825.83 1 149.81 -6.33 641.06 1 116.29 289.43 10 286.63 6 68.25 2.80 4 4820.98 30

P-value (Prob. > F) < 0.000 < 0.000 < 0.000 < 0.006 0.015 0.227 0.157 0.574 0.174 0.450 0.946 0.681 0.527 0.354 0.155 0.853 < 0.003 < 0.013 < 0.015 < 0.000 < 0.000 < 0.001

Std Dev. = 2.34; Mean = 52.95; C.V.% = 3.57; PRESS = 590.63; R 2 = 0.9400; Adj. R2 = 0.8200; Predicted R2 = 0.8006; Adeq. Precision = 17.001; S = 0.2471. To determine the adequacy of the models depicting the removal of alumina by the dissolution of Ukpor clay in hydrochloric acid, two different tests, i.e. the sequential model sum of squares and the model summary statistics, were conducted. The corresponding results are tabulated in Table 5. The results from the sequential model indicated that the 2FI model did not provide a good description of the experimental data. From the model summary statistics, it can be seen that the “Predicted R2” of 0.8006 was in reasonable agreement with the “Adjusted R2” of 0.8200 for the quadratic model. Furthermore, the quadratic model had maximum “Predicted R2” and “Adjusted R2” values. The afore-mentioned results indicate that the quadratic model provided an excellent explanation for the relationship between the independent variables and the corresponding response.

Source

Sum of squares Sequential model sum of squares Linear 2288.65 2FI 271.85 Quadratic 1971.05 Cubic 119.05 Source

Standard Deviation Model summary statistics Linear 6.54

Table 5: Adequacy of the Model Tested Degree of Mean squares F-value freedom

P-value

Remarks

5 10 5 15

457.73 27.19 394.21 7.94

15.81 0.94 13.62 3.20

0.000 0.538 < 0.000 0.0244

Significant Not significant Significant Significant

R2

Adjusted R2

Predicted R2

PRESS

Remarks

0.3436

0.2578

0.2919

2054.01

Inadequate

735 | P a g e

R. O. Ajemba and O. D. Onukwuli / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 5, September- October 2012, pp.732-742 2FI

7.39

0.3802

0.0897

0.1720

2336.00

Quadratic

2.35

0.9400

0.8200

0.8006

590.63

Cubic

1.58

0.9694

0.9086

0.6205

788.48

signal Inadequate signal Adequate signal Inadequate signal

The data were also analyzed to check the correlation between the experimental and predicted dissolution yield (Y %), as shown in Fig. 1. The experimental values were the measured response data for the runs designed by the CCRD model, while the predicted values were obtained by calculation from the quadratic equation. It can be seen from Figure 1 that the data points on the plot were reasonably distributed near to the straight line (R 2 = 0.9400), indicating a good relationship between the experimental and predicted values of the response, and that the underlying assumptions of the above analysis were appropriate.

Predicted

80.5 0

73.0 8

65.6 5

58.2 2

50.8 0 50.8 0

58.2 2

65.6 5

73.0 8

80.5 0

Actua l

Figure 1: Predicted values versus the experimental values.

% Yield

The main effects of the process variables on the response variable are plotted in Fig. 2. The figure shows that increasing the calcination temperature, leaching temperature, and acid concentration increases the % yield, while solid/liquid ratio and stirring speed has no statistical significant effect on the response and should be held constant at the center values.

67 59 51 43 35 Calcina t

Dissolu t

Acid con

Solid/l i

Stirrin g

Figure 2: Main effects plot of the process variables. 3.3. Response surface plots The three-dimensional response surface plots, obtained as a function of two factors maintaining all other factors constant at the mid-values, are helpful in understanding both the main effects and the interaction effects of these

736 | P a g e

R. O. Ajemba and O. D. Onukwuli / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 5, September- October 2012, pp.732-742 five factors. The corresponding contour plots, represented by the projection of the response surfaces in the x-y plane, provide a straightforward determination of the effects of the independent variables on the dependent variable. The three-dimensional response surface plots and related contour plots obtained are depicted in Figs. 3 to 14. Fig. 3 shows the dependency of alumina yield on calcination temperature and leaching temperature. Alumina yield increased with increase in calcination temperature to about 730 0C and thereafter yield remained constant with further increase in Calcination temperature, this is in agreement with the findings of Ata et al, [14]. The same trend was observed in Figs. 4 to 6. Increase in leaching temperature resulted in increase in alumina yield up to 1070C and thereafter decreased gradually. This is evident from Figs. 4, 7, 8 and 9. Low levels of solid/liquid ratios resulted in higher % yield as shown in Figs. 6, 9, 11, and 12.

82

Y ie ld

79

76

73

70

120.00

800.00 105.00

700.00 90.00

B: Leach Temp

600.00 75.00

500.00 60.00

400.00

A: Cal Temp

Figure 3: 3D plot showing the effect of calcination temp and leaching temp. on % yield.

82

Y ie ld

78.5

75

71.5

68

4.00

800.00 3.13

700.00 2.25

C: Acid conc

600.00 1.38

500.00 0.50

400.00

A: Cal Temp

Figure 4: 3D plot of the effect of calcination temp and acid concentration on % yield.

737 | P a g e

R. O. Ajemba and O. D. Onukwuli / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 5, September- October 2012, pp.732-742

81

Y ie ld

78

75

72

69

720.00

800.00 562.50

700.00 405.00

D: Stirring Rate

600.00 247.50

500.00 90.00

400.00

A: Cal Temp

Figure 5: 3D plot of the effect of calcination temp and stirring rate on yield.

82

Y ie ld

79

76

73

70

0.04

800.00 0.03

700.00 0.03

E: Solid/Liquid Ratio

600.00 0.02

500.00 0.02

400.00

A: Cal Temp

Figure 6: 3D plot of effect of calcination temp and solid/liquid ratio on % yield.

738 | P a g e

R. O. Ajemba and O. D. Onukwuli / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 5, September- October 2012, pp.732-742

82

Y ie ld

78.75

75.5

72.25

69

4.00

120.00 3.13

105.00 2.25

C: Acid conc

90.00 1.38

75.00 0.50

60.00

B: Leach Temp

Figure 7: 3D plot of leaching temp and acid concentration on % yield.

81

Y ie ld

78.25

75.5

72.75

70

720.00

120.00 562.50

105.00 405.00

D: Stirring Rate

90.00 247.50

75.00 90.00

60.00

B: Leach Temp

Figure 8: 3D plot of the effect of leaching temp and stirring rate on % yield.

739 | P a g e

81

Y ie ld

78

75

72

69

0.04

120.00 0.03

105.00 0.03

E: Solid/Liquid Ratio

90.00 0.02

75.00 0.02

60.00

B: Leach Temp

Figure 9: 3D plot of the effect of leaching temp and solid/liquid ratio on % yield.

81

Y ie ld

77.75

74.5

71.25

68

720.00

4.00 562.50

3.13 405.00

D: Stirring Rate

2.25 247.50

1.38 90.00

0.50

C: Acid conc

Figure 10: 3D plot of the effect of acid concentration and stirring rate on % yield.

740 | P a g e

81

Y ie ld

77.75

74.5

71.25

68

0.04

4.00 0.03

3.13 0.03

E: Solid/Liquid Ratio

2.25 0.02

1.38 0.02

0.50

C: Acid conc

Figure 11: 3D plot of the effect of acid concentration and solid/liquid ratio on % yield.

81

Y ie ld

78.25

75.5

72.75

70

0.04

720.00 0.03

562.50 0.03

E: Solid/Liquid Ratio

405.00 0.02

247.50 0.02

90.00

D: Stirring Rate

Figure 12: 3D plot of the effect of stirring rate and solid/liquid ratio on % yield.

741 | P a g e

R. O. Ajemba and O. D. Onukwuli / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 5, September- October 2012, pp.732-742 3.4.

Numerical Optimization One of the primary objectives of the present study was to find the optimum process parameters for maximizing the dissolution of Ukpor clay in hydrochloric acid solution. The model capable of predicting the maximum dissolution capacity showed that the optimum values of the process variables were a calcination temperature of 668.540C, a leaching temperature of 107.220C, an acid concentration of 2.93 mol/l, a stirring rate of 368.24 rpm, and a solid/liquid ratio of 0.027g/ml. Under these conditions, the predicted dissolution % yield was 97.85, which was in good agreement with the experimental value of 97.67%.

[6]

[7]

[8]

4. CONCLUSION The optimum levels of the process parameters for the dissolution of Ukpor clay in hydrochloric acid solution were investigated in this work using response surface methodology. Highly accurate model developed showed that the percentage yield of alumina from Ukpor clay was influenced by calcination temperature, leaching temperature, acid concentration, stirring speed and solid/liquid ratio. The optimum leaching conditions of alumina recovery from Ukpor clay are 668.54 0C calcination temperature, 107.22 0C leaching temperature, 2.93 mol/L acid concentration, 368.24 rpm stirring speed, and 0.027 g/ml solid/liquid ratio and under these conditions about 97.85% of the alumina content of the clay sample would have been removed. The above results show that Ukpor clay is a good source for alumina and the method employed is efficient for maximum production.

[9]

[10]

[11]

[12]

REFERENCES [1]

[2]

[3]

[4]

[5]

Abali Y., Colak S., Yapici S., “The optimization of the dissolution of phosphate rock with Cl2-SO2 gas mixture in aqueous medium,” Hydrometallurgy, 46, 1997, 27 – 35. Abali Y., Salih B., Kadir A., Ali V., Optimization of dolomite ore leaching in hydrochloric acid solutions, Physicochemical Problems of Mineral Processing, 46, 2011, 253 – 262. Veglio F., Ubaldin S., Optimization of pure stibnite leaching conditions by response surface methodology, European Journal of Mineral Processing & Environmental Protection, 1 (2), 2001, 103 – 112. Uzun D., Gulfen M., Dissolution of iron and aluminium from red mud in sulphuric acid solution, Indian Journal of Chemical Technology, 14, 2007, 263 – 268. Numluk P., Chaisena A., Sulphuric acid and ammonium sulphate leaching of

[13]

[14]

alumina from Lampang clay, E-Journal of Chemistry, 9(3), 2012, 1364 – 1372. Abdulwahab A., Suad A., Alumina recovery from Iraqi kaolinitic clay by hydrochloric acid route, Iraqi Bulletin of Geology & Mining, 2 (1), 2006, 67 – 76. Zafar I. Z., Ashraf M., Reaction kinetic model for dissolution of low grade bauxite rock in sulphuric acid, Journal of Chemical Society of Pakistan, 30 (1), 2008, 49 – 54. Lai-shi L., Yu-sheng W., Ying-ying L., Yu-chun Z., Extraction of alumina from coal fly ash with sulphuric acid leaching method, The Chinese Journal of Process Engineering, 11 (2), 2011, 254 – 258. Li D., Park K., Wu Z., Guo X., Response surface design for nickel recovery from laterite by sulfation-roasting-leaching process, Transactions of Nonferrous Metallurgy Society of China, 20, 2010, s92 – s96. Narayana S. K., King P., Gopinadh R., Sreelakshmi V., Response surface optimization of dye removal by using waste prawn shells,” International Journal of Chemical Sciences & Applications, 2 (3), 2011, 186 – 193. Yartasi A., Copur M., Ozmetin C., Kocakerim M., Temur H., An optimization study of dissolution of oxidized copper ore in NH3 solutions, Energy Education, Science and Technology, 3, 1999, 77. Shyi-Liang S., Hwang L., Process optimization of vacuum fried carrot chips using central composite rotatable design, Journal of Food & Drug Analysis, 19 (3), 2011, 324 – 330. Box G. E. P., Hunter W. G., and Hunter J. S., Statistics for experimenters: an introduction to design, data analysis and model building, (Wiley and Sons, New York, 1978). Ata O. N., Colak S., Ekinci Z., Copur M., Determination of the optimum conditions for the dissolution of stibnite in HCl solution, Chemical and Biochemical Engineering Quarterly, 24, 2001, 409.

742 | P a g e